In this study, by using an equivalent circuit method, a polarization-insensitive terahertz (THz) absorber based on multilayer graphene-based metasurfaces (MGBMs) is systematically designed, providing an extremely broad absorption bandwidth (BW). The proposed absorber is a compact, three-layer structure, comprising square-, cross-, and circular-shaped graphene metasurfaces embedded between three separator dielectrics. The equivalent-conductivity method serves as a parameter retrieval technique to characterize the graphene metasurfaces as the components of the proposed circuit model. Good agreement is observed between the full-wave simulations and the equivalent-circuit predictions. The optimum MGBM absorber exhibits $>90\%$ absorbance in an extremely broad frequency band of 0.55–3.12 THz ($\mathrm{BW}=140\%$). The results indicate a significant BW enhancement compared with both the previous metal- and graphene-based THz absorbers, highlighting the capability of the designed MGBM absorber. To clarify the physical mechanism of absorption, the surface current and the electric-field distributions, as well as the power loss density of each graphene metasurface, are monitored and discussed. The MGBM functionality is evaluated under a wide range of incident wave angles to prove that the proposed absorber is omnidirectional and polarization-insensitive. These superior performances guarantee the applicability of the MGBM structure as an ultra-broadband absorber for various THz applications.

You do not have subscription access to this journal. Citation lists with outbound citation links are available to subscribers only. You may subscribe either as an Optica member, or as an authorized user of your institution.

You do not have subscription access to this journal. Cited by links are available to subscribers only. You may subscribe either as an Optica member, or as an authorized user of your institution.

You do not have subscription access to this journal. Figure files are available to subscribers only. You may subscribe either as an Optica member, or as an authorized user of your institution.

You do not have subscription access to this journal. Article tables are available to subscribers only. You may subscribe either as an Optica member, or as an authorized user of your institution.

You do not have subscription access to this journal. Equations are available to subscribers only. You may subscribe either as an Optica member, or as an authorized user of your institution.

Parameters of Designed MGBM Absorber with Three Circular-shaped Graphene Metasurfaces^{a}

$p$

${E}_{f1}$

${\tau}_{1}$

${r}_{1}$

${E}_{f2}$

33 μm

0 ev

0.05 ps

10 μm

0.1 ev

${\tau}_{2}$

${r}_{2}$

${E}_{f3}$

${\tau}_{3}$

${r}_{3}$

0.2 ps

14.5 μm

0.65 ev

0.1 ps

15.5 μm

The indexes of 1, 2, and 3 refer to the top, middle, and bottom layers, respectively. The optimum thicknesses are extracted as ${t}_{1}=4\text{\hspace{0.17em}}\mathrm{\mu m}$, ${t}_{2}=16\text{\hspace{0.17em}}\mathrm{\mu m}$, and ${t}_{3}=30\text{\hspace{0.17em}}\mathrm{\mu m}$ (${t}_{\text{total}}=50\text{\hspace{0.17em}}\mathrm{\mu m}$).

Table 2.

Parameters of Designed MGBM Absorber withThree Cross-Shaped Graphene Metasurfaces^{a}

$p$

${E}_{f1}$

${\tau}_{1}$

${w}_{1}$

${E}_{f2}$

73 μm

0.14 ev

0.1 ps

27 μm

0.15 ev

${\tau}_{2}$

${w}_{2}$

${E}_{f3}$

${\tau}_{3}$

${w}_{3}$

0.4 ps

23 μm

0.9 ev

0.15 ps

32 μm

The indexes of 1, 2, and 3 refer to the top, middle, and bottom layers, respectively. The optimum thicknesses are extracted as ${t}_{1}=8.5\text{\hspace{0.17em}}\mathrm{\mu m}$, ${t}_{2}=12\text{\hspace{0.17em}}\mathrm{\mu m}$, and ${t}_{3}=29.5\text{\hspace{0.17em}}\mathrm{\mu m}$ (${t}_{\text{total}}=50\text{\hspace{0.17em}}\mathrm{\mu m}$).

Table 3.

Parameters of Designed MGBM Absorber with Three Square-Shaped Graphene Metasurfaces^{a}

$p$

${E}_{f1}$

${\tau}_{1}$

${a}_{1}$

${E}_{f2}$

23.5 μm

0.1 ev

0.2 ps

6 μm

0.3 ev

${\tau}_{2}$

${a}_{2}$

${E}_{f3}$

${\tau}_{3}$

${a}_{3}$

0.1 ps

23 μm

0.4 ev

0.2 ps

15 μm

The indexes of 1, 2, and 3 refer to the top, middle, and bottom layers, respectively. The optimum thicknesses are extracted as ${t}_{1}=9.5\text{\hspace{0.17em}}\mathrm{\mu m}$, ${t}_{2}=15\text{\hspace{0.17em}}\mathrm{\mu m}$, and ${t}_{3}=25.5\text{\hspace{0.17em}}\mathrm{\mu m}$ (${t}_{\text{total}}=50\text{\hspace{0.17em}}\mathrm{\mu m}$).

Table 4.

Optimum Parameters for the Extremely Broadband MGBM Absorber^{a}

$p$

${E}_{f1}$

${\tau}_{1}$

$r$

${E}_{f2}$

58.3 μm

0.37 ev

0.25 ps

12.95 μm

0.35 eV

${\tau}_{2}$

$w$

${E}_{f3}$

${\tau}_{3}$

$a$

0.1 ps

14 μm

0.85 eV

0.1 ps

54 μm

The indexes of 1, 2, and 3 refer to the circular-, cross- and square-shaped metasurfaces, respectively.

Table 5.

Comparison of the Designed MGBM Absorber with Similar Broadband THz Absorbers Previously Reported

$\lambda $ refers to the wavelength of the minimum frequency of the operating band.

Tables (5)

Table 1.

Parameters of Designed MGBM Absorber with Three Circular-shaped Graphene Metasurfaces^{a}

$p$

${E}_{f1}$

${\tau}_{1}$

${r}_{1}$

${E}_{f2}$

33 μm

0 ev

0.05 ps

10 μm

0.1 ev

${\tau}_{2}$

${r}_{2}$

${E}_{f3}$

${\tau}_{3}$

${r}_{3}$

0.2 ps

14.5 μm

0.65 ev

0.1 ps

15.5 μm

The indexes of 1, 2, and 3 refer to the top, middle, and bottom layers, respectively. The optimum thicknesses are extracted as ${t}_{1}=4\text{\hspace{0.17em}}\mathrm{\mu m}$, ${t}_{2}=16\text{\hspace{0.17em}}\mathrm{\mu m}$, and ${t}_{3}=30\text{\hspace{0.17em}}\mathrm{\mu m}$ (${t}_{\text{total}}=50\text{\hspace{0.17em}}\mathrm{\mu m}$).

Table 2.

Parameters of Designed MGBM Absorber withThree Cross-Shaped Graphene Metasurfaces^{a}

$p$

${E}_{f1}$

${\tau}_{1}$

${w}_{1}$

${E}_{f2}$

73 μm

0.14 ev

0.1 ps

27 μm

0.15 ev

${\tau}_{2}$

${w}_{2}$

${E}_{f3}$

${\tau}_{3}$

${w}_{3}$

0.4 ps

23 μm

0.9 ev

0.15 ps

32 μm

The indexes of 1, 2, and 3 refer to the top, middle, and bottom layers, respectively. The optimum thicknesses are extracted as ${t}_{1}=8.5\text{\hspace{0.17em}}\mathrm{\mu m}$, ${t}_{2}=12\text{\hspace{0.17em}}\mathrm{\mu m}$, and ${t}_{3}=29.5\text{\hspace{0.17em}}\mathrm{\mu m}$ (${t}_{\text{total}}=50\text{\hspace{0.17em}}\mathrm{\mu m}$).

Table 3.

Parameters of Designed MGBM Absorber with Three Square-Shaped Graphene Metasurfaces^{a}

$p$

${E}_{f1}$

${\tau}_{1}$

${a}_{1}$

${E}_{f2}$

23.5 μm

0.1 ev

0.2 ps

6 μm

0.3 ev

${\tau}_{2}$

${a}_{2}$

${E}_{f3}$

${\tau}_{3}$

${a}_{3}$

0.1 ps

23 μm

0.4 ev

0.2 ps

15 μm

The indexes of 1, 2, and 3 refer to the top, middle, and bottom layers, respectively. The optimum thicknesses are extracted as ${t}_{1}=9.5\text{\hspace{0.17em}}\mathrm{\mu m}$, ${t}_{2}=15\text{\hspace{0.17em}}\mathrm{\mu m}$, and ${t}_{3}=25.5\text{\hspace{0.17em}}\mathrm{\mu m}$ (${t}_{\text{total}}=50\text{\hspace{0.17em}}\mathrm{\mu m}$).

Table 4.

Optimum Parameters for the Extremely Broadband MGBM Absorber^{a}

$p$

${E}_{f1}$

${\tau}_{1}$

$r$

${E}_{f2}$

58.3 μm

0.37 ev

0.25 ps

12.95 μm

0.35 eV

${\tau}_{2}$

$w$

${E}_{f3}$

${\tau}_{3}$

$a$

0.1 ps

14 μm

0.85 eV

0.1 ps

54 μm

The indexes of 1, 2, and 3 refer to the circular-, cross- and square-shaped metasurfaces, respectively.

Table 5.

Comparison of the Designed MGBM Absorber with Similar Broadband THz Absorbers Previously Reported